|Monthly Tech-Tip |
These two Plainsman M370 mugs were fired at cone 6, the left one with G2934 matte glaze, the right one with G2934Y4 matte. They look and feel identical in the hand. The two glazes have the same chemistry. But they employ different materials to source that chemistry. The secret of of the matteness is high MgO (magnesia content). In the glaze on the left that MgO is sourced by dolomite, a lot of it. The glaze on the right sources it from a special frit, Ferro 3249. The impact of this difference is visible in the melt flows, the fritted one is obviously melting and flowing better. On other clays, especially stonewares, the G2934 can have a dry surface that cutlery marks. Thicker applications make it worse. But the Y version exhibits no such issues. Its mattness, durability, cleanability and hardness are so good that it is being used in floor tile.
Ceramic glazes melt and flow according to their chemistry and mineralogy. Observing and measuring the nature and amount of flow is important in understanding them.
G2934Y - Cone 6 Magnesia Matte Low LOI Version
The same chemistry as the widely used G2934 but the MgO is sourced from a frit and talc instead of dolomite. It has a finer surface, less cutlery marking and staining.
G2934Y variations for fired hardness, COE adjustment, less crawling, etc
G2934Y is a popular recipe used worldwide in industry and by potters and hobbyist. This page shows it, and four variations, that adjust for different purposes. All have the same chemistry, but source the needed oxides from different materials.